Добавил:
Upload Опубликованный материал нарушает ваши авторские права? Сообщите нам.
Вуз: Предмет: Файл:
Composite Materials for Aircraft Structures.pdf
Скачиваний:
443
Добавлен:
31.05.2015
Размер:
9.22 Mб
Скачать

42 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

i

i

 a) b) c) Fig. 2.12 Possible composite tensile failure modes: a) fiber bundle; b) crack; c) statistical. For carbon fibers in an epoxy matrix,/3 ~ 10 and 6 = 10 -2 m m (about a fiber diameter), so if L = 100 mm, then: 6"B~ = { 100 "~1/10 \ 1 0 - 2 ) _-__2.5

This is the strengthening obtained by composite action.

# 2.6 Simple Estimate of Compressive Strength

The previously introduced equations relating to tensile failure do not apply to compressive strength because fibers do not fail in simple compression. Rather, they fail by local buckling. The actual behavior is very complicated because, to the external stresses, it is influenced by the presence of residual stresses in the matrix caused by the difference between fiber and matrix expansion coefficients. It has been shown, for example, that glass fibers in an epoxy matrix can buckle simply after cooling down from the resin cure temperature. As may be expected, when it is assumed that the fibers act as circular columns on an elastic foundation, the wavelength of the buckling increases with the fiber diameter.

Two pure buckling modes can be envisaged (See Fig. 2.14): 1) the shear mode in which the fibers buckle in-phase and the matrix is sheared or 2) the extensional mode, in which the matrix is stretched and compressed in an out-of-phase manner. The most likely mode is that producing the lowest energy in the system. While mixed modes are possible, they require more energy than do either of the pure modes.

 BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 43

Cross-sectional laye r of N fibers

Y

Cylindrical specimen of n layers (n = L/(~)

Fig. 2.13 Rosen's model showing chain of fiber bundles.

Analysis of the buckling ~is based on the energy method in which the change in strain energy of the fibers AUf and of the matrix AUm is equated to the work done AWby the external loads as the composite changes from the compressed but unbuckled state to the buckled state.

 m U f --~ A U m = A W (2.26)

In the model, the composite is considered two-dimensional, the fibers are treated as plates normal to the plane of Figure 2.15 (rather than rods), and the buckling pattern is assumed to be sinusoidal. The resulting buckling stress for the extensional mode is:

2 [ VfEmEf "]1/2

OVcmax ~

and for the shear mode:

Gm

 O ' c m a x - - - - (2.28) ( 1 - r e )

44 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

!

 IT I I a) b)

Fig. 2.14 Two pure buckling modes for unidirectional composites in compression: a) shear or in-phase mode; b) extension or out-of-phase mode.

As Vftends to zero, o¥ m a x for the extensional mode tends to zero; but, as Vftends

 to unity, ~rc m a x for the extensional mode becomes very large compared with O'cm a x for the shear mode. Thus, the extensional mode would be expected to apply for only small Vf. Assuming Ef>>Em and Vm= 1/3, with G m -~-Em/ 2(1 + v,,), then the transition occurs at (Em/lOEf)1/3, or at Vf= 10% for Ef/ E,n = 100, and at Vf = 22% for Ef/Em = 10.

It has been found that these equations overpredict the compressive strength considerably. In the case of boron/epoxy, the actual compressive strength is about 63% lower than that predicted, while for other material combinations the prediction can be worse. Generally the problem is that the predicted failure strains are much higher than the matrix yield strain. As an approximation to the inelastic behavior, the theory was expanded (Ref. 10) using a gradually reducing matrix shear modulus. This gives more reasonable agreement with experimental results.

A very simple approach that appears to predict the experimental behavior in some cases is obtained by assuming failure occurs when the matrix reaches its yield stress o-y. Thus, at failure:

 O'cmax = o'f V f --}.-o'YmV m (2.29)

where the fiber stress is given by strain compatibility as:

 Of= Em = (2.30)
 BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 45

/Y//

 i l \ ! / I i

(

 !i ¢! \ t1

/

I

Fig. 2.15 Model for buckling fibers in a unidirectional composite.

taking ey for an epoxy resin as 0.02 and Ef = 70 GPa for glass fibers, then

o-f = 0.02 x 70 GPa = 1.4 GPa

and so:

O'c" = trfVf = 1.4 x 0.6 = 0.84 GPa

(ignoring the small contribution from the matrix).

This result is in more reasonable agreement with typically observed values.

2.7Off-Axis Strength in Tension

The failure o f an orientated, but still unidirectional composite can be envisaged as occurring in any o f three modes:

(1)Failure normal to the fibers (as occurs with straight tension in the fiber direction)

(2)Failure parallel to the fibers by matrix rupture or fiber/matrix interface tensile failure

46 COMPOSITEMATERIALSFORAIRCRAFTSTRUCTURES

(3) Failure by shear o f the matrix or fiber/matrix interfacelf the fibers make an angle 4> with the direction o f applied tensile stress o-, then, as shown in Figure 2.16, the stresses can be resolved as follows:

 Tensile stress parallel to fibers ~rl = O'CO S 2 ~b Tensile stress normal to fibers o'2 = ~rsin2 4> Shear stress parallel to fibers T12 = V2o-sin 2~b

If ~ , ~ and r u represent the composite strengths in direct tension (0b = 0°), transverse tension (4> = 90°), and shear (~b = 45°), respectively, then the failure stress for each mode can be expressed as:

 Mode 1: o - COS2 Mode 2: o - - sin2 ~b (2.31) Mode 3: 2z. ~ r - - - -

sin 24>

Thus, the failure mode changes with ~b as shown in Figure 2.17. Although these results are obeyed quite well for many systems and the observed fracture modes

 / // IF=oA F / / /
 Fp = F cos ¢ Ap = A / sin ¢ FT = F s i n ¢ A T = A / c o s ¢

I F = a A

Fig. 2.16 Resolution of forces and areas in off-axis tension.

 BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 47 ~ e = Ol u /cos2¢

a = 2 xU/sin 2 \$

55 0 ' e

275

u / sin2

0

 0 10 20 30 &0 50 60 70 80 90

(degrees)

Fig. 2.17 Example of the variation of tensile strength versus orientation for a unidirectional composite.

are as predicted, the interaction of stresses and the occurrence of mixed-mode fractures are not accounted for. Ref. 1 presents a more detailed analysis that accounts for the complex stress states.

Figure 2.17 shows that strength falls rapidly with increasing 4,. However, if the plies are placed at + 4' and - 4', the rate of fall-off is very much less, even to values of 4' as high as 30 °. The reasons for this are intuitively obvious because the plies reinforce each other against mode 1 or mode 2 failure.

2.8 FractureToughness of Unidirectional Composites

2.8.1 Fracture Surface Energy

A measure of the toughness, or the resistance of a material to crack propagation, is its fracture surface energy 3,. This is defined as the minimum amount of energy required to create a unit area of free surface (crack) and is

48 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES

usually given in units of kJ m -2. Because two free surfaces are produced, R (for crack resistance) equal to 2T is the term often employed in fracture calculations.

It is a matter of considerable importance that, for crack propagation normal to the fibers (Fig. 2.18a), the fracture energy of a composite consisting of brittle fibers in a brittle matrix is usually much greater than is predicted by a simple rule-of-mixtures relationship. In general, R1 >> VfRf + VmRm.For example, in the case of a typical carbon/epoxy composite, Rm ~ 1 kJ m -2 for the bulk epoxy resin and Rf~ 0.1 kJ m -2 for the carbon fiber. However, the fracture surface

L_

 a) 1

q

c)

Fig. 2.18 Three basic modes of crack propagation in unidirectional fiber composites subject to simple tensile loading: a) normal to the fibers; b) parallel to the fibers; and c) crack deflection along the fibers, or splitting. Modes a and b are self-similar modes of propagation.

 BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 49

energy of a unidirectional composite Rc (if the crack is forced to propagate normal to the fibers) is typically 2 5 - 5 0 kJ m -2.

In contrast, for crack propagation parallel to the fibers (Fig. 2.18b), the fracture surface energy R2 is of the order of Rm if the crack propagates solely through the matrix; however R m will be lower if the crack propagates partially through the weaker fiber/matrix interface. Because R2 << R1, crack propagation parallel to the fibers, or splitting (Fig. 2.18c), will generally result even when the starting crack is normal to the fibers.

Considering crack propagation normal to the fibers (Fig. 2.18a), the total work of fracture can be attributed to a number of sources 11'1~ as shown in Figure 2.19 and Table 2.1 taken from Ref. 11. In the case of the brittle fiber/brittle matrix composite (Fig. 2.19a), crack growth proceeds by pulling fibers out of the matrix behind the crack front and by fracturing fibers ahead of the crack tip. Energy is absorbed during pull-out if the shear stress at the fiber/matrix interface is maintained while the fracture surface is separating. I f the fiber/matrix interface is relatively weak, local stresses will cause the fibers to be debonded from the matrix, with a resultant loss of stored strain energy. Stored strain energy is also lost by stress relaxation over the transfer length when the fiber fractures. Finally, strain energy is also lost from the fiber by crack bridging if the fiber spans the opening crack before fracture.

If the matrix is ductile, as in a metal-matrix composite, energy is also absorbed by matrix plastic deformation. This situation is illustrated in Figure 2.19b for the case in which the fiber is strongly bonded to the matrix so that little fiber pull-out

O c c u r s .

The work of the fracture contribution for pull-out in Table 2.1 refers to short constant-strength fibers. The expression would have to be modified for a statistical flaw distribution in continuous fibers. The contribution due to creation of new surfaces of fibers and matrix can be ignored in brittle systems, as can contributions from the matrix yield.

2.8.2Fracture Mechanics

The energetic requirement for crack propagation is that the energy-release rate (equal to the "fixed grips" strain energy release rate) G must equal the fracture surface energy R. At the critical condition,

 G = Gc = R (2.32)

In many cases, it is more convenient to work in terms of the stress intensity factor K. For an isotropic material in the crack opening mode, K/, is related to G through the equation K2 = EG and K2c = E G c at failure.

In the simple case of a small centre crack in a sheet under tension:

 /(l = o'('lra)1/2 (2.33)

50 COMPOSITEMATERIALS FOR AIRCRAFT STRUCTURES

FIBERS MATRIX

 CRACK -- ~ \ " ~ "
 FIBERS MATRIX t \,. / / . //:: ~/.,. %,, | %" : i "S; / i , " . / x ¢ ; FIBER BREAK, • , ,2,, I "~': <'Z PLASTIC ZONE C R A C K - " db.l,:;;I ~ i / , e V " • : : : ~'; ../,:I

/ J

N

/ /

b)

Fig. 2.19 F r a c t u r e behavio r durin g failure o f a) a brittle fiber/brittl e matri x composite an d b) a brittle fiber/ductil e m a t r i x composite where the fibers a r e assumed to be strongly bonded to the matrix .

 BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 51 Table 2.1 Models for Contributions to W o r k of Fracture for a Discontinuous Fiber Composite, Take n from Ref. 11 l*luuci "y II I^~I^ 1 Pull-out (short fibers of length L) Vfo~f82 - ~ (L > 28) Vf°'~fL2(L< 2a) 248 Debonding Vf(o~f)2y 4Ef Stress relaxation < Vf(o~f)28 3Ef - Crack bridging 2Vfr(~ff) 3 (1 - vf)(1 - 2vf) - - X 12(1 - vf) "fiEf Matrix plastic deformation (1 - Vf)2 aurarx vl x U ~m

where tr is the applie d stress and 2a the crack length. Thus, the stress trF at failure is given by

 trF = (2.34)

which is the familia r Griffith equation. 13

A relationship betwee n G and K can also be obtained for a fiber composit e materia l by m o d e l l i n g it as a continuous linear orthotropic material with the crack propagatin g on one o f the planes o f symmetry . Usin g the analysis for such

materials given in Ref. 14,

2 J L ,a,l/ k 2a,1 e l

Here the aij terms are the coefficients o f the stresses in the stress-strain law defined using a coordinate system based not on the fiber direction, but on the crack in the "1 direction" and the loa d in the "2 direction". This seems to be conventional in fracture mechanics treatments o f this type. The factor involving the a terms can be considered as the reciprocal o f the effective modulus E' o f the composite. F o r the simple case illustrated in Figure 2.18a, where the crack is perpendicular to the fiber direction:

 1 1 1 a22 -- E l l a l l = E22 a66 = 612 a12 - - 1)12 1)21 E11 E22
 52 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES taking as values typical of a carbon/epoxy composite, E l l = 140GPa, E22 ~-- 12 GPa, G12 = 6 GPa, v12 = 0.25, and v21 = 0.0213, then E' , ~ 0.4Ell. If,

alternatively, the crack is considered to lie parallel to the fibers (Fig. 2.18b), then E t ~ 2E22 where E' substitutes for the a terms in equation (2.35).

As long as crack propagation occurs on a plane of symmetry, the relationship between K1, O', and a for the linear orthotropic material remains the same as that for the isotropic material. Thus, referring back to the unidirectional composite, for a given crack length c~ and normal stress tr, a crack parallel to the fibers produces a larger G than one normal to the fibers. This results from the lower compliance of the composite when stressed in the fiber direction.

In the fiber composite material, the orientation dependence of R must also be taken into consideration. In general, a composite is notch-sensitive to cracks running parallel to the fibers (Fig. 2.18b) and the fracture mechanics principles described above may be directly employed. However, the composite may not be notch-sensitive in the situation shown in Figure 2.18a. In some cases,7 the composite may become notch-sensitive when a >> 8, the ineffective length, because the strain concentration in the matrix may then lead to fiber fractures at the crack tip. The crack would then become more effective with increasing a, as required in fracture mechanics considerations. However, in other cases, gross failure of the fiber/matrix interface may occur, resulting in the splitting mode of failure illustrated in Figure 2.18c. This situation, which occurs in more weakly bonded composites, results in complete notch-insensitivity (failure at the net section strength). Both of these situations are illustrated in some experimental work on carbon/epoxy composites in Figure 2.20, taken from Ref. 11.

The conditions for crack turning or splitting can be approached from energy considerations. 15 For the cracking illustrated in Figure 2.18c to occur in a unidirectional composite, it is necessary that:

 G] R1 < (2.36) G2 R2

where GliS the energy release rate for self-similar propagation and G2 the release rate for splitting. Typically, for carbon/epoxy R1/R2 is in the range 2 5 - 5 0 and

G1/G2 is about 20, so splitting is generally predicted.

As mentioned earlier, most advanced composite structures are made of laminates in the form of unidirectional plies laminated together at various orientations. The fracture behavior of these materials is considered in Chapter 6 and 8. In laminates, toughness is highly dependent on the degree of ply splitting and inter-ply disbonding (delamination), resulting in high-energy absorption and crack deflection.

An approach similar to that just described can be taken for this highly complex situation. 16 The direction of crack growth is based on the R1/R2ratio for each ply

and the G1/G2ratio for the laminate. The energy release rates are calculated by finite element procedures and recalculated after each increment of crack growth until the point of catastrophic failure.

Тут вы можете оставить комментарий к выбранному абзацу или сообщить об ошибке.

Оставленные комментарии видны всем.

Соседние файлы в предмете [НЕСОРТИРОВАННОЕ]